Microsoft Word - Gheorghe2016BT.docx34 Revista Român de Materiale / Romanian Journal of Materials 2016, 46 (1),34 -42
IN MEMORIAM Prof. Dr. Ing. PETRU BALT
MODELE EXPERIMENTALE DE MATERIALE COMPOZITE, CU CAPACITATE POTENIAL DE ÎNCAPSULARE A DEEURILOR
CU NIVEL SCZUT DE RADIOACTIVITATE EXPERIMENTAL MODELS OF GROUT TYPE COMPOSITE MATERIALS,
WITH POTENTIAL CAPACITY OF LOW LEVEL RADIOACTIVITY WASTES ENCAPSULATION
NASTASIA SACA1, LIDIA RADU1, CLAUDIU MAZILU1, MARIA GHEORGHE∗,
IONELA PETRE2, VIOREL FUGARU3 1Technical University of Civil Engineering, 122-124 Lacul Tei Bvd., sector 2, Bucharest, România
2CEPROCIM, 6 Preciziei Bvd., sector 6, Bucharest, România 3IFIN-HH, Str. Reactorului no.30, P.O.BOX MG-6, Bucharest – Mgurele, Bucharest, România
The main objective of this work is to identify,
based on experimental physical characteristics investigation, the grout types with potential capacity of residual radionuclides stabilization into storage container of low level radioactivity waste (LLW).
The grouts matrix based on Portland cement or special cement with lead slag addition and various fillers (limestone, L or pulverized fly ash, PFA) were carried out with river fine sand or lead slag recycled fine sand. The Portland cement /PFA or L ratios have had values of 30/70; 50/50 and 70/30, and cement/sand ratio was of 1/1.
There were tested on the physical characteristics – fluidity which assesses the filling ability of the LLW storage container, the density which reflects radionuclide shielding capacity, the shrinkage correlated with the microcracking potential and mechanical strengths evolution required of the long time secure LLW management.
Obiectivul principal al acestei lucrri este de
a identifica, pe baza datelor experimentale de investigare a caracteristicilor fizice, tipurile de grout cu capacitate potenial de stabilizare a radionuclizilor reziduali în containerul de stocare a deeurilor solide cu nivel redus de radioactivitate (LLW).
Grouturile cu matrice de ciment Portland sau ciment special cu adaos de zgur plumbic, i diferite filere (calcar, cenu zburtoare) s-au realizat cu nisip natural sau cu nisip reciclat (de zgur plumbic). Raportul ciment Portland /cenu sau filer de calcar a fost de 30/70; 50/50 i 70/30, iar raportul ciment/nisip a fost de 1/1. Au fost testate caracteristicile fizice - fluiditatea care evalueaz capacitatea de umplere a containerului cu deeuri solide LLW, densitatea ca msur a capacitii de ecranare la radionuclizi, contracia corelat cu potenialul de fisurare i evoluia rezistenelor mecanice, cerut pentru gestionarea în siguran, pe termen lung, a LLW. Modificrile microstructurale i elementale ale matricei pe baz de ciment cu zgur plumbic au fost investigate prin analiza SEM-EDAX.
Keywords: grout, special cement, lead slag, pulverised fly ash, encapsulation, low level radioactivity waste 1. Introduction
The developing of technological and functional performance of advanced composites for encapsulation / immobilization of radioactive waste with cumulated ability of ionizing radiation absorption/shielding is derived from necessity to protect health and the environment in the context of increasing impact nuclear technology in various applications and volume of radioactive waste.
The stabilization-solidification of radioactive waste process principle consists of encapsulate of solid waste, solidify liquid waste (included tritiated water), stabilise contaminated soils, stabilize tank- heel residues after tanks are emptied, and as low permeability barriers  Processing and immobilization of radioactive waste includes the operations that change physico-chemical characteristics such as pretreatment, treatment and conditioning. The conditioning may or may not
include immobilization. Immobilisation reduces the potential for migration or dispersion of radionuclides. As according to IAEA  immobilization is defined as conversion of waste into a waste form by solidification, embedding or encapsulation.
The radioactive wastes are stabilized by converting the radionuclides to a less mobile form as a result of various physico - chemical process as adsorption and chemical reactions, but the waste solidifying improves their mechanical performances. There are required for facilitate of handling, transportation storage and safety disposal of radioactive waste [1 - 3].
The grouts research materials proposed for research are advanced composite materials of functional type because they can provide special functions in the application. In this category are the selfcompacting grouts with LLW encapsulating/ immobilizing capacity.
∗ Autor corespondent/Corresponding author, E-mail: [email protected]
N. Saca, L. Radu, C. Mazilu, M. Gheorghe, I. Petre, V. Fugaru / Modele experimentale de materiale compozite, cu capacitate 35 potenial de încapsulare a deeurilor cu nivel sczut de radioactivitate
The main objective in managing and disposing of radioactive (or other) waste is to protect people and the environment. In July 2011 the European Union adopted a directive for the disposal of used nuclear fuel and radioactive wastes which requires member countries to develop national waste management plans for European Commission review by 2015 .
Ionizing radiations include alfa rays, beta rays, protons, neutrons, gamma rays and X rays which cause ionisation when passing through the matter, and is specifically divide into direct ionizing radiation and indirect ionizing radiation. In particular, gamma rays, X-rays or neutrons directly act on atoms or molecules, thus changing the main structure of DNA or proteins. When this type of radiation acts on the generative cell of a living organism, a probability for inducing mutation to thus bring about malformation and malfunction may be increased. The radioactive wastes require a appropriate system for radionuclides immobilizing by solidification/stabilisation into impermeable grout matrix and concrete barrier towards radionuclides diffusion. Also, the the area to which radiation is applied essentially requires a radiation shielding system able to shield gamma rays, X- rays or neutrons harmful for human body and environment . Low level wastes (LLW) contain radioactive materials where activity does not exceed 4 GBq/te of alpha or 12 GBq/te of beta/gamma [6, 7]. Intermediate level wastes (ILW) where radioactivity levels exceed those for LLW, but where heating is not an issue for storage or disposal facilities. The encapsulating/immobilizing into impermeable grouts is a appropriated method recommended and used in LLW and ILW radioactive waste disposal [8 - 10]. The method effective is due to compositional and functional modeling ability to achieve the set performance level. The grout main component is the cement and the high density, inert and pozzolanic or cementitious powder.
The grouts matrices are used as carriers for the radiation shielding composite materials and offer desired engineering and thermal attributes for various radiation management applications [8-11]. Properties of the cement and additives of grouts determine the long term durability of the protective material, the key property of these encapsulation systems. Many research projects are aimed for improving the durability of cement based composites as radioactive waste encapsulation or shielding systems by appropriate modification [11-16].
An upgraded solution for the existing technology of LLW encapsulation is proposed with a new advanced composite materials compatibles ensuring long term radionuclide confination. The main self-compacting grouts (SCG) technical characteristics are high fluidity and segregation stability, capacity to fill the narrowest spaces between comminuted LLW, and very low gas and liquid permeability of hardened state. The functional characteristics are described by the matrix compatibility with the LLW, due to solidification/stabilization (immobilization) capacity, of radionuclide from LLW solid and liquid with long life time.
In this context the paper presents the grout compositional factors influence on the structure and on the physical characteristics, appropriated to radioactive solid wastes encapsulation such as ensure the stability of the solidified wastes into container. The studied main characteristics which determine radionuclide diffusion transfer are:
- Fluidity, filling ability, stability of segregation and bleeding.
- Density. - Dimensional stability on long term. - Mechanical strengths evolution.
The obtaining and testing model of grout for LLW encapsulation, developed in this work, is schematic showed in Figure 1.
Fig 1 - Model of obtaining and testing of grout for LLW encapsulation/ Model experimental de obi- nere i testare a grouturilor pentru încap- sularea deeurilor cu radioactivitate sczut
36 N. Saca, L. Radu, C. Mazilu, M. Gheorghe, I. Petre, V. Fugaru/ Experimental models of grout type composite materials, with potential capacity of low level radioactivity wastes encapsulation
Table 1 The characteristics of blended cements with lead slag content
Caracteristicile cimenturilor cu adaos de zgur plumbic
The chemical composition (average values) of pulverised fly ash /Compoziia chimic (valori medii) a cenuii zburtoare
Content/Coninut SiO2 Al2O3 Fe2O3 CaO MgO SO3 Na2O K2O PC S Sulfides/ Sulfuri
Pulverised fly ash
52.0 24.7 7.9 8.6 2.3 0.9 0.7 1.4 1.8 0.13
SR EN 450 > 70% > 5 < 4 < 3 < 1 < 2.4 < 3 -
Characteristics/Caracteristica ZPb1-2 ZPb1-3 Density/Densitate, g/cm3 3.30 3.35 Blaine specific surface area/Suprafaa specific Blaine, cm2/g 4100 4090 /Water for standard consistency/Ap de consisten standard, % 24.0 24.9 Setting time/Timp de priz Initial/Inceput >8 h
Final/Sfârit < 24 h Stability/Stabilitate, mm 0.5 4.0 Cement type/Clasa de rezisten 42.5N 32.5R
2. Experimentals 2.1 Materials
The matrix of grouts contains two types of cements: CEM II/A-V 42.5N (provided by Lafarge Romania) and specially blended cements with slag lead addition of 20% (ZPb1-2) and 30% (ZPb1-3), obtained by CEPROCIM. The physical characteristics of cements with lead slag addition are presented in Table 1.
The grouts contain two types of mineral powders: pulverized fly ash (PFA) and limestone filler (L) which partially substitute the cement. The oxidic composition of PFA is given in Table 2.
Limestone filler used in grouts have the following characteristics: % CaO-53.5%, residue on 0.125 mm sieve- 9.8%, density-2700kg/m3.
The used superplastifiants admixtures (SP) were based on the modified carboxilated polyethers provided by Chryso and noted as SP1, SP2.
Lead primary slags (ZPb) were supplied by former ROMPLUMB S.A. dump. The ZPb was the secondary product of lead obtaining process. There are few areas of primary lead slag recovery as addition into cementitious grout and concrete. There are not identified in our country work of primary lead slag valorization in grouts and concretes, but exist attempts referring to inorganic polymers .
The ZPb used in this research were characterized by various content of lead and copper. The ZPb contains 6.6% PbO and 4.6% CuO. The lead primary slag was used as addition in cement and also as substitute of the fine sand in grout mix. The main mineralogical components of lead slags, determined by X-ray diffraction, were marganosite (Ca2PbSi3O9), gehlenite (Ca2Al[AlSiO7]) and quartz (SiO2). The ZPb was grinded and used as substitute of fine river sand. The characteristics were: density-3850 kg/m3, bulk density- 1880 kg/m3 and water absorption-0.4%. 2.2 Grout mixes
Blended cement based on the partial
replacement of Portland cement by secondary materials is currently used for encapsulation of radioactive waste. Up to 75% PFA is employed in encapsulation grouts, which is much higher values than those used in the construction industry. These percentages are selected to help reduce the heat released during cement hydration and avoid thermal cracking [18, 19].
This principle has been applied to the design of grout mixes based on secondary resources as partial substitutes of Portland cement or of river sand. The design of grout mixes was based on the modelling principle refering to rheological characteristics and compactity required by effective LLW encapsulation. The self compacting grouts are characterised by filling ability of the smalest gapes into containers with stored solid LLW. In this context, were carried out various grout mixes refering to type of components and their weight ratios.
2.2.1. The grout mixes with limestone filler and
pulverised fly ash The grout mixes are showed in the Tables 3-5.
The grout mixes contain cement type CEM II/A-V 42.5N and limestone filler or PFA as partial cement substitutes. The Portland cement /PFA or L ratios have values of 30/70; 50/50 and 70/30. The grout mixes are showed in Table 3.
2.2.2. The grout mixes with lead slag
The grout mixes contain primary lead slag both as blended cement addition and substitute of fine river sand. The lead slag led to the grout density required for a better shielding capacity at ionizing radiation. According with the obtained research results referring to L and PFA mixes were carried out two groups of lead slag grout mixes with powder/ZPb sand ratio of 30/70 and, respectively, of 50/50.
The first group of grout mixes with cement/filler ratio of 70/30, powder/ ZPb sand ratio of 30/70, water/powder ratio of 0.5 and SP1 of 1.6% is presented in Table 4.
N. Saca, L. Radu, C. Mazilu, M. Gheorghe, I. Petre, V. Fugaru / Modele experimentale de materiale compozite, cu capacitate 37 potenial de încapsulare a deeurilor cu nivel sczut de radioactivitate
Table 3 The grout mixes with limestone filer (L) and pulverised fly ash (PFA) as partial cement substitute
Compoziia grouturilor cu filer de calcar i cenu zburtoare ca substitueni ai cimentului Code CEM II/A-V 42.5N, % L,% PFA,% Water/Cement ratio/
Raport A/C Water/Power weight ratio/ Raport
1 P3V7 30 70 1.67 0.5 1.6 2 P5V5 50 50 1 0.5 1.6 3 PV2 70 30 0.7 0,5 1.6 4 P3C7 30 70 1.67 0.5 1.6 5 P5C5 50 50 1 0.5 1.6 6 PC2 70 30 0.7 0.5 1.6
The grout mixes with lead slag as recycled fine sand/ Compoziia grouturilor cu nisip reciclat de zgur plumbic Code CEM II/A-V
ZPb 0-1mm, % 1-2mm, %
1 Reference/GR referina 100 10 90 2 GC 70 30 10 90 3 GV 70 0 30 10 90
The grout mixes with lead slag as addition to blended cement and lead slag as recycled fine sand Compoziia grouturilor cu ciment cu adaos de zgur plumbic i nisip reciclat de zgur plumbic
Cement/ Ciment L, %
GR1 100 - - - - 90 10 - - 0.5 GC1 70 - - 30 - 90 10 - 0.71 GV1 70 - - - 30 90 10 - 0.71 GRN 100 - - - - 45 - 45 10 0.5 GZ2 - 100 - - - - - 90 10 0.5 GZ3 - 100 - - - - 90 10 0.5
The second group of grout is characterized by the cement/filler ratio of 70/30, powder/ ZPb sand ratio of 50/50, water/powder ratio of 0.5 and SP1 of 1.6% is presented in Table 5.
2.3 Methods 2.3.1. The cement-superplastifiant compatibility
The cement-superplastifiant compatibility (C-SP) consist of assessment of correlations between paste viscosity decreasing and type and content of SP admixture. The viscosity is influenced by the C3A and alkaline sulfate content in cement and specific surface. The SP is compatible with cement whether leads to fluidity increasing simultaneous with water/cement ratio decreasing. Also, cement-SP compatibility is emphasized by keeping constant paste initial consistency for a long time period. The cement– superplasticizer compatibility can be investigated by measuring realized flow time of grout as according with several researches [20-22]. The cement paste fluidity usually is represented by a curve indicating the flow time C–SP system according to superplasticizer dosage at various times. Saturation superplasticizer dosage corresponding to a break in the curve when superplasticizer is added over the saturation point; it does not improve any more the fluidity of C–SP but only increases the risk of sedimentation and
delays the cement setting time. The C-SP compatibility was carried out as
following: - Establishment of the minim standard
consistency water at various SP amounts of the ZPb cement type.
- Measuring of the flow time of the paste by con Marsh method.
Grout mixes as fresh and hardened state were monitored for: fluidity, segregation resistance and bleeding, setting time, dimensional stability and cracking and compressive strength. The grout compressive strength acceptance criterion for secure LLW encapsulation is minim 10 MPa at 28 days. The bending strength testing is need as information about cracking potential. The dimensional stability and the mechanical strengths were tested on 4x4x16 cm samples. All values presented in the paper are the average value of three determinations.
The microstructure of the some hardened grouts was described by SEM method. 3. Results 3.1 The cement-SP compatibility
The results of lead slag cement-SP compatibility are graphically showed in Figure 2. The minimum water amount for standard consistency into range of 17...18% were obtained at the 1.7…1.8% SP content.
38 N. Saca, L. Radu, C. Mazilu, M. Gheorghe, I. Petre, V. Fugaru/ Experimental models of grout type composite materials, with potential capacity of low level radioactivity wastes encapsulation
Fig. 2 - The compatibility of the blended cements with lead slag with HRWR superplasticizer/Compatibilitatea cimenturilor cu adaos de zgur de plumb cu aditivul superplastifiant puternic reductor de ap.
Fig 3 - The variation of flow time versus superplasticizer,
tested at water/cement ratio of 0.5/ Variaia fluiditii, ca timp de curgere, în funcie de aditivul superplastifiant, la raport A/C=0.5
The cement type CEM II/A-V 42.5N is
characterised by flow time values according to experimental data graphically showed in the Figure 3.
The C-SP compatibility was investigated for two SP types of admixtures appart to carboxilated polyethers class. It is found the minimum flow time values are different depending on SP type at the same saturation concentration of 1.6...1.8% range values. Thus, the SP1 is more efficient than SP2., because the flow time was of 25 s and, respectively, 48 s at the same saturation concentration of the 1.6% .
3.2 The characteristics of the fresh grouts
The compositional influences factors were verified by testing of engineering self compacting grouts. These characteristics are controlled by the mix parameters such as powder types and cement/addition ratios, water/cement (powder)
ratio, cement/sand ratio and SP admixture. The characteristics of different mix design grouts are briefly presented in Table 6.
The fluidity of grouts measured as flow time through Marsh funnel (aperture diameter of 10 mm) varied with grout mix design namely type of cement, filler (limestone or pulverized fly ash) and sand (river sand or recycled lead slag).
The PFA influences the fluidity in the compositional context meaning the powder type. Thus, the PFA increase the flow time (viscosity) in cement-PFA system in comparison with cement- limestone filler system. The increasing of filler content modified grout viscosity. Increasing the content of PFA from 30% to 50% and, respectively, 70% in cement-PFA system leads to significant increasing of grout flow time from 70 to 500 seconds, although the water/cement ratio was from 0.7 to 1.67. The grout P5V5 is distinguished by higher resistance of segregation and bleeding than the others. The high content PFA grouts maintain initially consistency a longer time than those with lower content of PFA.
Different behavior was observed at cement-limestone filler couple; increased of limestone content insignificantly decreased the flow time (from 18 to 8 seconds) at the same values of W/C ratio with cement-PFA couple.
The obtained results showed that the fluidity of the grout decreases with the introduction of the fillers, this reduction is proportional to their replacement level and type, according to data obtained by other authors [20- 22].
The experimental grout fluidity values as flow times were significantly influenced by the content and fineness of lead slag. The recycled lead slag as fine sand in grout mix leads to increasing of the fluidity. Thus, the increasing of lead slag fine sand from 50 to 70 % resulted in constantly decreasing of flow time. The obtained values were influenced by the other factors namely filler type (limestone or PFA) and water/cement ratio. The results are showed in Table 7.
The data referring to grout mixes of powder/ZPb recycled sand ratio of 30/70 lead to the following:
- The cement-limestone couple had the fluidity very good (flow time of 8 seconds) appropriated to encapsulate by confining of the solid LLW.
Table 6 The characteristics of the fresh grouts with limestone filler and fly ash
Caracteristicile grouturilor cu filer de calcar i cenu zburatoare, în stare proapt
Flow time/Timp de curgere, s Unit weight/Masa volumic, kg/m3
N. Saca, L. Radu, C. Mazilu, M. Gheorghe, I. Petre, V. Fugaru / Modele experimentale de materiale compozite, cu capacitate 39 potenial de încapsulare a deeurilor cu nivel sczut de radioactivitate
Table 7 The characteristics of the fresh grouts with lead…